Thin Solid Films 453 – 454 (2004) 36–41 0040-6090/04/$ - see front matter 2003 Elsevier B.V. All rights reserved. doi:10.1016/j.tsf.2003.11.156 Microstructuring of glassy carbon: comparison of laser machining and reactive ion etching M. Kuhnke , Th. Lippert *, E. Ortelli , G.G. Scherer , A. Wokaun a a, b a a Paul Scherrer Institut, 5232 Villigen, Switzerland a Dyconex AG, 8303 Bassersdorf, Switzerland b Abstract Structuring of glassy carbon (GC) can be performed by various methods such as sawing, laser ablation, and reactive ion etching (RIE). Laser machining with a tripled Nd:YAG laser at an irradiation wavelength of 355 nm allows the fabrication of V- shaped channels with depths )600 mm and aspect ratios )5. This method is very flexible for rapid prototyping, but is comparatively slow due to the sequential machining. A complete flowfield consisting of 100 parallel channels with a depth of 250 mm and a top width of 50 mm was prepared by direct laser ablation and tested in a micro fuel cell. As an alternative, a novel process combining laser structuring of a metal mask with subsequent reactive ion etching was developed. The quality of the metal layer and the ablation behavior are strongly influenced by the metal adhesion, which depends on the GC pretreatment and the deposition technique. Reactive ion etching of glassy carbon can be performed with etch rates of f40 mmh , but the y1 high pressure conditions of 100 mTorr (0.13 mbar) limit the aspect ratio to -1.5 due to pronounced underetching. The fabrication of structures with aspect ratios )4 and etch rates of f10 mmh is possible with the use of alternative etching devices with y1 different design or plasma sources. 2003 Elsevier B.V. All rights reserved. Keywords: Glassy carbon; Micro fuel cell; Laser ablation; Metal film; Reactive ion etching 1. Introduction Fuel cells are a promising technology for energy conversion, and have recently gained attention in the sector of small power supplies for portable applications such as notebooks, camcorders, and cell phones. For these applications, a miniaturized cell design was devel- oped that reduces the number of components and sim- plifies manufacturing and assembly. A main component of this miniaturized cell is an electrode made from glassy carbon (GC, Sigradur G, pyrolyzed at 2200 K) that contains a channel structure with typical dimensions of 50 mm width and 200 mm depth. This flowfield provides the gas supply, a support for the electrocatalyst, and allows one to study the mechanisms that determine catalyst utilization. Several techniques for the fabrication of structures in GC have been studied in our group. The simplest *Corresponding author. Tel.: q41-56-310-4076; fax: q41-56-310- 4412. E-mail address: [email protected](T. Lippert). technique is sawing of the structures with a wafer saw, resulting in channels with a rectangular cross section (15=150 mm) and a maximum aspect ratio of 10 w1,2x. Unfortunately, this method is very slow due to the sequential machining, and only straight channels reach- ing from one sample edge to the other can be fabricated. Therefore, an additional sealing of the cell for the gas distribution is required. Another technique for structuring GC is direct laser ablation that can be performed with pulsed UV lasers w3x. This method is very flexible for rapid prototyping of different flowfield layouts, when a computer con- trolled xyz stage or a galvano scanner are used. This is also a sequential technique, but the application of a laser with a kHz repetition rate permits comparably fast processing. The fabricated channels have a V-shaped cross-section with maximum aspect ratios of f5. A novel method for the structuring of glassy carbon is the combination of a laser ablation step with subse- quent reactive ion etching. In this process, a metal layer is deposited on the glassy carbon and structured by laser ablation, in order to create a mask for the reactive ion
Thin Solid Films 453–454(2004) 36–41
0040-6090/04/$ - see front matter� 2003 Elsevier B.V. All rights reserved.doi:10.1016/j.tsf.2003.11.156
Microstructuring of glassy carbon: comparison of laser machining andreactive ion etching
M. Kuhnke , Th. Lippert *, E. Ortelli , G.G. Scherer , A. Wokauna a, b a a
Paul Scherrer Institut, 5232 Villigen, Switzerlanda
Dyconex AG, 8303 Bassersdorf, Switzerlandb
Structuring of glassy carbon(GC) can be performed by various methods such as sawing, laser ablation, and reactive ionetching(RIE). Laser machining with a tripled Nd:YAG laser at an irradiation wavelength of 355 nm allows the fabrication of V-shaped channels with depths)600 mm and aspect ratios)5. This method is very flexible for rapid prototyping, but iscomparatively slow due to the sequential machining. A complete flowfield consisting of 100 parallel channels with a depth of250 mm and a top width of 50mm was prepared by direct laser ablation and tested in a micro fuel cell. As an alternative, anovel process combining laser structuring of a metal mask with subsequent reactive ion etching was developed. The quality ofthe metal layer and the ablation behavior are strongly influenced by the metal adhesion, which depends on the GC pretreatmentand the deposition technique. Reactive ion etching of glassy carbon can be performed with etch rates off40 mm h , but they1
high pressure conditions of 100 mTorr(0.13 mbar) limit the aspect ratio to-1.5 due to pronounced underetching. The fabricationof structures with aspect ratios)4 and etch rates off10 mm h is possible with the use of alternative etching devices withy1
different design or plasma sources.� 2003 Elsevier B.V. All rights reserved.
Keywords: Glassy carbon; Micro fuel cell; Laser ablation; Metal film; Reactive ion etching
Fuel cells are a promising technology for energyconversion, and have recently gained attention in thesector of small power supplies for portable applicationssuch as notebooks, camcorders, and cell phones. Forthese applications, a miniaturized cell design was devel-oped that reduces the number of components and sim-plifies manufacturing and assembly. A main componentof this miniaturized cell is an electrode made fromglassy carbon(GC, Sigradur G, pyrolyzed at 2200 K)�
that contains a channel structure with typical dimensionsof 50 mm width and 200mm depth. This flowfieldprovides the gas supply, a support for the electrocatalyst,and allows one to study the mechanisms that determinecatalyst utilization.
Several techniques for the fabrication of structures inGC have been studied in our group. The simplest
technique is sawing of the structures with a wafer saw,resulting in channels with a rectangular cross section(15=150mm) and a maximum aspect ratio of 10w1,2x.Unfortunately, this method is very slow due to thesequential machining, and only straight channels reach-ing from one sample edge to the other can be fabricated.Therefore, an additional sealing of the cell for the gasdistribution is required.
Another technique for structuring GC is direct laserablation that can be performed with pulsed UV lasersw3x. This method is very flexible for rapid prototypingof different flowfield layouts, when a computer con-trolled xyz stage or a galvano scanner are used. This isalso a sequential technique, but the application of a laserwith a kHz repetition rate permits comparably fastprocessing. The fabricated channels have a V-shapedcross-section with maximum aspect ratios off5.
A novel method for the structuring of glassy carbonis the combination of a laser ablation step with subse-quent reactive ion etching. In this process, a metal layeris deposited on the glassy carbon and structured by laserablation, in order to create a mask for the reactive ion
37M. Kuhnke et al. / Thin Solid Films 453 –454 (2004) 36–41
etching step. The structuring step can be very fast,because the metal film thickness is only a few hundrednanometers, and it provides the same flexibility as thelaser ablation process. The pattern of this mask is thentransferred into the glassy carbon substrate by a RIEstep in oxygen plasmaw4,5x. RIE chambers have a quitelarge working area, e.g. 6 inches in diameter that allowsparallel structuring of up to 70 GC electrodes(sizeincluding flow field and gas supply: 14=14 mm). Thecarbon is gasified by the reactive oxygen species withan additional support by the ion bombardment.
2.1. Set-up for direct laser ablation of GC
Laser ablation of glassy carbon was performed withXeCl (308 nm) and ArF (193 nm) excimer lasers andwith a diode-pumped Nd:YAG laser(frequency tripled:355 nm). Round or square spots with a size of 20–60mm were ablated by imaging a pin hole on the samplesurface with a lens(fs10 cm). The sample wasmounted on a computer controlledxyz stage while theposition of the laser beam was fixed.
For the fabrication of the micro fuel cell flow fields,a tripled Nd:YAG with 8 kHz repetition rate, whichcannot be obtained by excimer lasers, was used tooptimize the fabrication speed. A pulse energy of 0.24mJ was imaged on a spot with a diameter of 20mm,corresponding to a fluence of 76.4 J cm . The sampley2
was moved with a speed of 76.8 mm s or 9.6mmy1
2.2. Devices for sample processing and processcharacterization
Different methods for pretreating the GC before proc-essing were characterized by determination of roughnessand electrical resistance, by XPS and SEM, and bycomparison of their effect on ablation properties. ADektak 8000 profilometer was used for determining theaverage roughness(arithmetic average, i.e. arithmeticalmean deviation of the profile) of the samples surfaces.The electrical resistance of the GC samples was meas-ured with a simple two-tip set-up where two gold tipswere pressed on the surface with a separation of 8 mmand a reproducible force.
The metal film was structured by pulsed laser ablationand 20:1 demagnification of a 1 mm pinhole onto thesubstrate surface. The ablation characteristics were deter-mined by varying the fluence in the range of 0.5–3.0 Jcm and the number of pulses between 1 and 100.y2
Line patterns were fabricated by step and repeat imaging.For the reactive ion etching of GC an Alcatel GIR300
with a glass-covered 6 inch electrode, a maximum RFpower of 600 W and a pressure range of 5–100 mTorr
(6.7=10 –1.3=10 mbar) were applied. Alterna-y3 y1
tively, an Oxford Instruments Plasmafab 100 RIE couldbe used.
3. Results and discussion
3.1. Pretreatment and determination of parameters
Before the micro structuring processes could beaccomplished, several stages had to be studied in moredetail.
Various methods have been tested for improving theadhesion of metal layers on GC, i.e. simple ultrasoniccleaning in solvents, reactive(O ) and non-reactive2
(Ar) ion etchingw6x, and polishing, that yields the bestresult. For a better understanding of the adhesion prop-erties, several characterization steps were performed oneach sample before and after pretreatment. In the follow-ing, a brief summary of these experiments is given.
The surface roughnessR of the untreated samplesa
was determined in order to see if higher or lowerroughness would be beneficial for the adhesion. Meas-urements show that the roughness of the untreatedsample (f75 nm) can be reduced to approximatelyone-third by ultrasonic cleaning in solvents or by etchingin O or Ar plasma. The higher roughness()90 nm)2
of the polished sample in combination with a greatreduction of craters seems to contribute significantly togood adhesion properties of the metal film.
The electrical resistance did not change significantlyafter solvent cleaning and increased byf20% after O2
plasma etching. After polishing, it increased byf80%,probably due to the oxidation of the surface, which wasobserved by XPS. The Ar plasma etched sample unex-pectedly exhibited the highest resistance, i.e.)2.5 timeshigher than the untreated sample. This result is evenmore surprising as the oxygen fraction of the surface,determined by XPS, is much lower than after O plasma2
treatment. The high resistances could partially resultfrom a considerable amount of silicon contamination ofthe substrate surfaces, probably originating from theglass covered RF electrode in the RIE device.
The most important criterion for the choice of thepretreatment method was the ablation behavior, wherethe polished sample exhibited the best properties, suchas defined ablation edges with low roughness and nometal film peeling in the non-irradiated areas.
3.3. Parameters for metal ablation
The ablation behavior of metal layers was comparedfor XeCl (308 nm) and ArF (193 nm) excimer lasers.The ablated spots with a diameter of 70mm were
38 M. Kuhnke et al. / Thin Solid Films 453 –454 (2004) 36–41
Fig. 1. Ablation spot in an Al film on GC, irradiated with 10 pulsesat 308 nm and 1.9 J cm (� 70 mm).y2
Fig. 2. Bulk ablation rate of glassy carbon at different wavelengths. The data labeled by(q) were obtained by Th. Kunzw1x.
studied by SEM after irradiation with 10 pulses. At lowfluences, i.e. approximately 0.5 J cm , melting and re-y2
solidification of the metal without significant ablation isobserved. In the range of 1.0–2.0 J cm , the metaly2
layer is almost completely removed and a zone of re-deposited Al is formed in the vicinity of the ablatedspot (Fig. 1). Further increase of the fluence results inthe formation of a ‘splash zone’ of molten and re-solidified Al around the spot. At a fluence of 2.0 Jcm , a nearly complete ablation is reached after twoy2
to three pulses. Fewer pulses lead to more Al particles
remaining in the ablation spot, pulse numbers abovef5can damage the metal layer surrounding the spot.
3.4. Parameters for glassy carbon ablation
The ablation properties of GC were studied in com-parison to the metal layer, because it is also etchedduring the metal structuring. The ablation rates andthreshold fluences of GC depend on the irradiationwavelength and were determined for XeCl and ArFlasers in the low fluence range(Fig. 2) with 1 Hzrepetition rate. Threshold fluences of-400 mJ cm aty2
193 nm andf1 J cm at 308 nm were determined byy2
logarithmic regression using Eq.(1):
B E1 FC Fd F s ln (1)Ž .D Ga Feff th
where dsablation depth, a seffective absorptioneff
coefficient,Fsfluence,F sthreshold fluencew7x.th
For fluences above 2 J cm , the ablation rate at 308y2
nm is f3.5 times higher than at 193 nm, probablycaused by plasma shielding, i.e. absorption of the VUVpulse by the created plasma. The effective absorptioncoefficients of glassy carbonw8x are 14.3"0.6 mm aty1
193 nm and 4.1"0.2 mm at 308 nm. Experimentsy1
performed by Kunz w9x with a XeCl laser andSigradur K (pyrolyzed at 1000 K) revealed a similar�
effective absorption coefficient of approximately 2.7mm and ablation rates of approximately 1.1mmy1
pulse at 20 J cm .y1 y2
39M. Kuhnke et al. / Thin Solid Films 453 –454 (2004) 36–41
Fig. 3. (a) Micro fuel cell electrode with a laser-machined flowfield and gas supply channels fabricated by electrical discharge machining.(b)SEM micrograph of flowfield channels, viewed from the supply channel, as indicated by the white arrow.
Fig. 4. Process flow scheme of the combined Laser-RIE-process. Each step(x) is explained in the text.
3.5. Laser machining of glassy carbon electrodes
Glassy carbon electrodes were laser-structured withthe frequency-tripled Nd:YAG(355 nm, 8 kHz). Thesimple fuel cell flow field fabricated in GC is 1 cm in2
size and consists of 100 parallel channels with a pitchof 100 mm and a length of 10 mm(Fig. 3a). Afterseven runs, V-shaped channels with a depth off250mm and a top width off50 mm were achieved(Fig.3b), corresponding to an aspect ratio of 5. The ablationrate is decreasing with increasing channel depth due toreflections at the channel walls and possibly due toredeposition of ablated material on the walls. An averageablation rate of 18mm pulse was obtained for they1
electrode shown in Fig. 3.A pair of electrodes was sputter-coated with platinum
and assembled with a Nafion membrane. This microfuel cell was tested with hydrogen and oxygen gas andproved that the principle is working. The cell was gastight up to)200 kPa and achieved a power of 2.5 mW.
3.6. Laser–RIE process
Due to the sequential nature of the laser process,alternative methods were developed, i.e. a combinationof a laser ablation step for the fabrication of a maskwith a reactive ion etching step for the glassy carbonetching. Fig. 4 shows a process flow scheme of thecomplete process steps.(1) The first step in this process is the pretreatment
of the glassy carbon sample, which ensures good adhe-sion of the metal film to the carbon. Polishing resultedin the best adhesion and ablation properties.(2) The second step is the deposition of the metal
film, which either consists of a single Al layer with 400nm thickness or can be supported by an additionaladhesion promoting Cr layer of 10 nm thickness. Ther-mal evaporation or sputtering can both be applied, butthe density and adhesion of sputtered films are higher,which was determined by measuring the thickness and
40 M. Kuhnke et al. / Thin Solid Films 453 –454 (2004) 36–41
Fig. 5. Line structures in an Al layer on GC with 60mmwidthyspacing.
Fig. 7. SEM micrograph of GC etched with an alternative RIE set-up.
Fig. 6. SEM micrograph of oxygen plasma etched GC; the mask is partially removed(indicated by the arrow).
transmission of the film. The sputtered films revealed alower transmission for a comparable thickness.(3) The metal film is then structured by pulsed laser
ablation with 2.0 J cm . Line structures for a masky2
were obtained by step and repeat processing with over-lapping ablation spots. Fig. 5 shows a 1.2=1.2 mm2
line pattern with a widthyspacing of 60mm. At a feedspeed of 20mm pulse , the resulting edge roughnessy1
wasf3 mm.(4) After patterning the etch mask, the sample was
etched with 1.1 W cm power(800 V bias) at 100y2
mTorr (0.13 mbar) pressure and 5 sccm oxygen flow.Channels with a depth of)70 mm and a top width of109 mm were obtained at an etch rate of)35 mm hy1
(Fig. 6). The picture shows strong underetching due to
the high-pressure applied in the experiment. With theseconditions, the sidewall angle isf198, correspondingto a maximum achievable aspect ratio of-1.5. Despitethe high bias voltage, the aluminum mask revealed agood durability and an acceptable etch rate off150mm h . The achieved selectivity, i.e. the ratio of they1
etch rates in GC and in Al, is in the range of 200–250.With a different RIE device(Oxford Instruments
Plasmafab 100), aspect ratios of)4 were reached atlower bias voltages and lower etch rates(f10 mmh , see Fig. 7). With the different chamber designy1
corresponding to a lower bias voltage, the etch rate waslower than in the Alcatel Instrument(at same conditionsof power, pressure and oxygen flow).(5) The last step is the removal of the metal mask by
wet chemical etching.
41M. Kuhnke et al. / Thin Solid Films 453 –454 (2004) 36–41
Laser ablation is a fast and simple technique for rapidfabrication of structures in GC, e.g. for prototypes ofmodel electrodes. Due to the sequential processing it isprobably not suitable for a commercial fabrication pro-cess. Deep V-shaped channels can be fabricated withhigh aspect ratios, but the channel bottoms are poorlydefined.
The novel process combining a laser ablation stepwith a reactive ion-etching step is more complicated butalso more flexible due to various parameters and proc-essing steps. One of the main advantages is the parallelprocessing of many samples at the same time, resultingin relatively cheap fabrication. Low aspect ratio struc-tures with depths of several hundred micrometers areeasy to achieve, but it is necessary to optimize theprocess to obtain high aspect ratio structures. More
sophisticated etching devices with higher plasma densityand lower bias voltage allow higher etch rates and lowermask degradation, resulting in aspect ratios)4.
w1x Th. Kunz, Dissertation, No. 12076, ETH, Zurich, 1997.¨w2x L. Pajasova, L. Soukup, L. Jastrabık, D. Chvostova, Surf. Rev.´ ´ ´
Lett. 9 (1) (2002) 473–477.w3x R. Srinivasan, B. Braren, Chem. Rev. 89(1989) 1303.w4x N.M.D. Brown, N. Cui, A. McKinley, Appl. Surf. Sci. 133
(1998) 157–165.w5x Y. Sohda, D.M. Tanenbaum, S.W. Turner, H.G. Craighead, J.
Vac. Sci. Technol. B 15(2) (1997) 343–348.w6x K. Popova, Vacuum 48(7–9) (1997) 681–684.w7x J. Wei, Dissertation, No. 13856, ETH, Zurich, 2000.¨w8x Z. Veziridis, Dissertation, No. 13397, ETH, Zurich, 2000.¨w9x U.A. Paulus, Z. Veziridis, B. Schnyder, M. Kuhnke, G.G.
Scherer, A. Wokaun, J. Electroanal. Chem. 541, 2003, pp.77–91.